Flexible Tricolor Flag-liked Microribbons Array with Enhanced Conductive Anisotropy and Multifunctionality

Anisotropically conductive materials are important components in subminiature devices. However, at this stage, some defects have limited practical applications of them, especially low anisotropic degree and high cost. Here, we report novel tricolor flag-liked microribbons array prepared by electrospinning technique. The tricolor flag-liked microribbons array is composed of parallel microribbons, and each microribbon consists of three different regions, just like tricolor flag. The tricolor flag-liked microribbons array is only electrically conductive in the direction parallel to the microribbons, whereas in the perpendicular and thickness directions are insulative. The electrical conductivity along parallel direction reaches up to 8 orders of magnitude higher than that along perpendicular direction. The degree of anisotropy in present study is increased by 2 orders of magnitude than that of the anisotropically conductive material in references reported before. Besides, other functions can be conveniently assembled into tricolor flag-liked microribbons array to realize multifunctionality. Owing to the high electrical anisotropy and multifunctionality, tricolor flag-liked microribbons array will have important applications. Furthermore, a universal technique to prepare microribbons with three functional regions has been established for fabricating excellent multifunctional materials.

conductivity along parallel direction was three times higher than that along perpendicular direction. Majewski, et al. 12 achieved anisotropic ionic conductivity in block copolymer membranes by magnetic field alignment. The conductivity along parallel direction of the membranes reached up to 1000 times higher than perpendicular direction. In year 2014, Huang, et al. 13 fabricated an anisotropic conductive polymer film by shear-flow inducing MWCNTs to assemble into well-ordered parallel MWCNT stripes vertical to the shear flow. The electrical measurement showed that the electrical resistivity along the MWCNT stripes was 6 orders of magnitude lower than that orthogonal to the stripes, which was the reported most striking conductive anisotropy for the plastic anisotropic conductive materials. Very recently, Liu, et al. 14 prepared highly aligned polyimide composite fibers film with graphene nanoribbon and carbon nanotube hybrids as nanofillers by means of electrospinning. The conductivity ratio between the parallel and perpendicular directions of the product also reached up to 6 orders of magnitude. On the basis of many literatures concerning anisotropically conductive materials, it can be noticed that how to effectively enhance the degree of anisotropy of anisotropically conductive materials is an important and urgent issue.
Electrospinning technique has been widely adopted to effectively fabricate 1D nano/micro materials [15][16][17][18][19][20][21][22][23] . The electrospun products have some unique advantages, such as long length (up to several meters), good flexibility (owing to the polymer template) and low power consumption. Furthermore, the order of the electrospun products can be arranged by using special collector [24][25][26][27] . In this work, we present a simple one-pot electrospinning method to acquire a new kind of anisotropically conductive material by using a specially designed spinneret. Our design concept for the novel anisotropically conductive material is to introduce two insulative regions on both sides of conductive region of a microribbon, and arrange the microribbons into parallel structure. The novel microribbons with three different regions were just like tricolor flag, and thus, we named the microribbons as tricolor flag-liked microribbons. Based on this structure, the conducting substance (PANI) can be effectively isolated by insulative regions in perpendicular direction, and thus, it is expected that very high conductive anisotropy can be achieved. Moreover, since multifunctionality of future materials is the development trend, establishing a universal method to assemble different components with various functions together becomes an meaningful subject of study. For the tricolor flag-liked microribbon, other non-conductive functional materials can be introduced into the two insulative regions to achieve versatility. In this work, we chose magnetic and photoluminescent materials as examples and respectively added them into the two insulative regions. Thus, the final tricolor flag-liked microribbons array not only possesses anisotropic conduction, but also photoluminescent and magnetic properties. Furthermore, it is feasible to replace these materials with other functional materials according to the application requirements to realize multifunctionality. From the viewpoint of multifunctional materials, the design concept and construction technique are of great significance to fabricate multifunctional micro/nano materials.

Preparation of oleic acid modified Fe 3 O 4 nanoparticles, Tb(BA) 3 phen complexes and PMMA.
Fe 3 O 4 nanoparticles with the saturation magnetization of 62.02 emu g −1 were obtained by using a facile coprecipitation synthetic method (see Electronic supplementary information) 28 . To improve the monodispersity, stability, and solubility of Fe 3 O 4 nanoparticles in the spinning solution, the as-prepared Fe 3 O 4 nanoparticles were coated with oleic acid as below: 1.5 g of the as-prepared Fe 3 O 4 nanoparticles were ultrasonically dispersed in 50 mL of deionized water for 20 min. The suspension was heated to 80 °C under an argon atmosphere with vigorous mechanical stirring for 30 min and then 0.5 mL of oleic acid was slowly added. The reaction was stopped after heating and stirring the mixture for 40 min. The precipitates were collected from the solution by magnetic separation, washed with ethyl alcohol for three times, and then dried in an electric vacuum oven at 60 °C for 6 h. Then, all of the products were used to prepare spinning solution III. Tb(BA) 3 phen powders were synthesized according to the traditional method as described in the literature 29 . PMMA used in this study was prepared by oxidative polymerization of MMA according to the reference 30.
Preparation of spinning solutions. Three different spinning solutions, respectively marked as I, II and III, were used to fabricate tricolor flag-liked microribbons array. The spinning solution I for the photoluminescent-insulative region consisted of Tb(BA) 3 phen, PMMA, CHCl 3 , and DMF. It has been known through our previous work that the optimum ratio of Tb(BA) 3 phen to PMMA is 1:10 28 . Thus for the preparation of the spinning solution I, 0.5000 g of PMMA and 0.0500 g of Tb(BA) 3 phen were added into the mixed solution of 9.3750 g of CHCl 3 and 0.6250 g of DMF under magnetic stirring for 48 h.
As for the preparation of spinning solution II for the conductive region, 0.5000 g of PMMA was dissolved into the mixed solution of 9.3750 g of CHCl 3  for 48 h. The mixture was then cooled down to 0 °C in an ice-bath. Then 0.1500 g of ANI and 0.1873 g of CSA were added into the above mixture and kept stirring for 2 h, followed by introducing 0.3676 g of APS for 30 min. The final mixture was allowed to react at 0 °C for 24 h. The impact of different amounts of ANI, CSA and APS on the conductivity of conductive region was discussed in Electronic supplementary information.
The spinning solution III for the magnetic-insulative region was composed of all the as-prepared oleic acid modified Fe 3 O 4 nanoparticles, 0.5000 g of PMMA, 9.3750 g of CHCl 3 and 0.6250 g of DMF. The mixture was firstly ultrasonically dispersed for 20 min and then stirred under mechanical agitation for 48 h.

Fabrication of tricolor flag-liked microribbons array.
A sketch of the modified electrospinning setup is illustrated in Fig. 1, and more detailed manufacture process and utilization of the specially designed spinneret are provided in Electronic supplementary information. In the electrospinning process, three different spinning solutions respectively marked as I, II and III were loaded into three syringes. When the three spinning solutions flowed down to the plastic nozzle, they would form a triple parallel structure. During this process, the three spinning solutions would not blend owing to their viscous resistance. Subsequently, the three spinning solutions were stretched by electric field force to form a jet with triple parallel structure. The jet was then stretched to ribbon shape by electrostatic repulsion and solidified with the volatilization of solvents, thus a microribbon with three different regions was obtained. In order to obtain tricolor flag-liked microribbons array, an aluminum rotary drum was used as a collector, which was put about 18 cm away from the tip of the plastic nozzle. The aluminum rotary drum was 20 cm in length, 7 cm in diameter, fixed in horizontal, and the rotation speed was 1500 r min −1 . A positive direct current (DC) voltage of 6 kV was applied between the spinneret and the collector to generate stable, continuous PMMA-based tricolor flag-liked microribbons array at room temperature of 20-22 °C and the relative humidity of 20-30%. Because the microribbon swung in the air due to the instability of electrospinning process, an array with a certain width could be collected on the surface of the aluminum rotary drum.
Characterization. The phase compositions were identified by an X-ray powder diffractometer (Bruker, D8 FOCUS) with CuKα radiation. The operation voltage and current were kept at 40 kV and 20 mA, respectively. The morphologies and internal structures were observed by a field-emission scanning electron microscope (FESEM, XL-30) and a biological microscope (BM, CVM500E), respectively. The elemental analysis was performed by an energy-dispersive spectrometer (Oxford Instruments) attached to the FESEM. The electrical properties were measured by a Hall effect measurement system (ECOPIA HMS-3000) and a dielectric spectrometer (Concept 80). The fluorescent properties were investigated by Hitachi fluorescence spectrophotometer F-7000. The UV-Vis absorption spectra were recorded by a UV-Vis spectrophotometer (SHIMADZU UV mini 1240). Then, the magnetic performances were measured by a vibrating sample magnetometer (VSM, MPMS SQUID XL). All the determinations were performed at room temperature.

Results and Discussion
Morphology and internal structure. Figure 2a displays a typical SEM image of the product. All the microribbons are aligned in the same direction, and the width of every single microribbon is ca. 10 μ m and the thickness is less than 1 μ m. Moreover, it can be seen that almost all the broadsides of these microribbons are facing up, with few exceptions, which is probably because this arrangement would help the microribbons lay in a more stable and lower potential energy state onto the aluminum rotary drum. The faced up orientation of broadsides for the microribbons can facilitate the isolation effect of insulative regions on the conductive region in perpendicular direction. Depending on the transmission light of optical microscope, the inner structures of the tricolor flag-liked microribbons can be observed. As revealed in Fig. 2b, a clear triple parallel structure, just like tricolor flag, can be seen in a microribbon: one side contains large quantities of tawny oleic acid modified Fe 3 O 4 nanoparticles, the middle part is scattered with green PANI, and another side is transparent. In order to further determine the structure of each single tricolor flag-liked microribbon, energy dispersive spectrum (EDS) in line scan mode was performed, where Fe, S and Tb elements represent Fe 3 O 4 , PANI and Tb(BA) 3 phen, respectively. As shown in Fig. 2c, elemental Fe, S and Tb respectively exist in one side, middle and another side part of a tricolor flag-liked microribbon. The EDS mapping tests shown in Fig. 2d-f also manifest the same result.
From the above results, we can safely conclude that a novel material with a new and interesting structure has been successfully fabricated. Figure 2g,h present the typical digital camera photos of the resulting tricolor flag-liked microribbons array. One can see that the tricolor flag-liked microribbons array can be freely bent and folded. This is critically important for the application of the material in the flexible device.
Electrical characteristics of tricolor flag-liked microribbons array. In order to investigate the anisotropic conductivity of the tricolor flag-liked microribbons array, a small piece of soldering tin was cut into four little pieces with diameter of ca. 2 mm and was pressed onto the sample (The sample has been cut into the size of ca. 3 cm × 3 cm × 0.5 mm), as indicated in Fig. 3a. Then the four pins of a Hall effect measurement system were respectively pressed on the four pieces of soldering tin. The relationships of voltage and current between P 1 and P 2 , P 3 and P 4 , P 2 and P 3 , P 1 and P 4 were recorded by Hall effect measurement system, and the results were presented in Fig. 3b. The determined electrical conductivity between P 1 and P 2 , P 3 and P 4 , P 2 and P 3 , P 1 and P 4 are listed in Table 1. One can see that the conductivity along parallel direction (P 1 -P 2 ; P 3 -P 4 ) is ca. 8 orders of magnitude higher than that along perpendicular direction (P 2 -P 3 ; P 1 -P 4 ), demonstrating that the tricolor flag-liked microribbons array has a strong anisotropy in conductivity. To the best of our knowledge, up to now, this value of conductivity ratio is the highest for anisotropically conductive materials.
The conductivity in the thickness direction of tricolor flag-liked microribbons array is also measured, by using a Concept 80 dielectric spectrometer. As seen in Fig. 3c, the measured conductivities are less than 4 × 10 −9 S cm −1 in an alternating current frequency range of 1 Hz to 100000 Hz, indicating that the tricolor flag-liked microribbons array is insulative in its thickness direction. From the above measurement results, we can conclude that the tricolor flag-liked microribbons array is only electrically conductive in the direction parallel to the ribbons, whereas in the perpendicular and thickness directions are insulative.
As described in some literatures 8,11 , anisotropic conductivity of an electrospun fibrous film can be attributed to the different electrical connection between parallel and perpendicular direction. Electrons can move without block through the fibers in parallel direction, whereas a lot of interfaces among the fibers hinder the movement of electrons to some extent in perpendicular direction. However, as previously mentioned, the conductivity ratios between parallel and perpendicular direction of the most of products reported in literatures are very low, meaning that the interfaces can not effectively hinder the movement of electrons in perpendicular direction. The schematic diagram of tricolor flag-liked microribbons array is shown Fig. 4, in which the left part reveals a multilayered structure, and the structure of a single tricolor flag-liked microribbon is also proposed, which has interesting structure, just like tricolor flag (we use a picture of French flag to illustrate). Regarding the tricolor flag-liked microribbons array, because the conductive region of each tricolor flag-liked microribbon is sandwiched between two insulative regions, and almost all the broadsides of the flag-liked microribbons are facing up, the conductive regions of the tricolor flag-liked microribbons are separated by the plenty of insulative regions in (b) I-V curves of the tricolor flag-liked microribbons array in the directions between P 1 and P 2 , P 3 and P 4 , P 2 and P 3 , P 1 and P 4 ; and (c) variation of conductivity in the thickness direction of tricolor flag-liked microribbons array with alternating current frequency.

Directions
Conductivity (S cm −1 ) P 1 -P 2 (6.45 ± 0.03) × 10 −4 P 3 -P 4 (6.20 ± 0.02) × 10 −4 P 2 -P 3 (1.21 ± 0.01) × 10 −12 P 1 -P 4 (1.35 ± 0.02) × 10 −12 Table 1. Conductivity between P 1 and P 2 , P 3 and P 4 , P 2 and P 3 , P 1 and P 4 . perpendicular direction, which further blocks the movement of electrons. As for the thickness direction, because the electrospun microribbons are landed randomly onto the aluminum rotary drum, the conductive region in a microribbon has little chance to align with the other conductive region in the lower layer. Once adequate number of layers is collected, statistically, the conductive regions are misaligned and not connective in thickness direction, and thus, the tricolor flag-liked microribbons array is insulated in its thickness direction. Figure  It is well known that the saturation magnetization of a magnetic composite material depends on the mass percentage of the magnetic substance in the magnetic composite material [28][29][30] . The saturation magnetization of the Fe 3 O 4 nanoparticles before coating by oleic acid is 62.02 emu g −1 , and the remanence nears zero (see Supplementary Figure S3). By using of the as-prepared Fe 3 O 4 nanoparticles, the tricolor flag-liked microribbons array shows its saturation magnetization of 9.80 emu g −1 and remanence of zero, as seen in Fig. 5b. The magnetic properties indicate that the tricolor flag-liked microribbons array possesses superparamagnetic property.

Multifunctionalization by introducing photoluminescence and magnetism.
The above analyses reveal that other functions, such as magnetism and photoluminescence, can be introduced into the insulative regions to realize multifunctionality of the tricolor flag-liked microribbons array, as long as the adopted materials do not compromise insulativity.

Conclusions
We have fabricated a new type of anisotropically conductive material which is named as tricolor flag-liked microribbons array via simple electrospinning technology. The obtained tricolor flag-liked microribbons array consists of parallel-arranged tricolor flag-liked microribbons, and each tricolor flag-liked microribbon is composed of three different regions, which are photoluminescent-insulative region, conductive region and magnetic-insulative region, respectively. The conductive region is sandwiched between photoluminescent-insulative region and magnetic-insulative region. Owing to this unique structure, the electrical conductivity along parallel direction is more than 8 orders of magnitude higher than that along perpendicular direction, and the thickness direction of the product is determined to be insulative. Meanwhile, we have demonstrated that other functions, such as magnetism and photoluminescence, can be assembled into the insulative regions to realize multifunctionality of the tricolor flag-liked microribbons array, as long as the adopted materials do not harm insulativity. More importantly, the design concept and fabrication technique for the tricolor flag-liked microribbons array provide a new and facile approach for preparing other anisotropic materials with multifunctionality.